Single Crystals of the Isotypic Series BaLu2Ch4 (Ch = S, Se and Te) with CaFe2O4-Type Structure
Schurz, Christian M.; Schleid, Thomas; Crystals 1 (2012) 78–86; doi:10.3390/cryst1030078

data_1508410
_publ_section_title
;
 Single Crystals of the Isotypic Series BaLu2Ch4 (Ch = S, Se and Te) with
 CaFe2O4-Type Structure
;
_journal_issue                   3
_journal_name_full               Crystals
_journal_page_first              78
_journal_page_last               86
_journal_paper_doi               10.3390/cryst1030078
_journal_volume                  1
_journal_year                    2012
_chemical_formula_sum            'Ba Lu2 Te4'
_chemical_formula_weight         997.68
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.5358(8)
_cell_length_b                   4.3847(3)
_cell_length_c                   15.9362(9)
_cell_measurement_reflns_used    35386
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      28.28
_cell_measurement_theta_min      0.41
_cell_volume                     945.82(10)
_computing_cell_refinement       'HKL Scalepack (Otwinowski & Minor 1997)'
_computing_data_collection       'Collect (Nonius BV, 1997-2000)'
_computing_data_reduction
'HKL Denzo and Scalepack (Otwinowski & Minor 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Kappa CCD (Nonius)'
_diffrn_measurement_method       CCD
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0938
_diffrn_reflns_av_sigmaI/netI    0.0612
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       5
_diffrn_reflns_limit_k_min       -5
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            17321
_diffrn_reflns_theta_full        28.28
_diffrn_reflns_theta_max         28.28
_diffrn_reflns_theta_min         1.97
_exptl_absorpt_coefficient_mu    36.832
_exptl_absorpt_correction_T_max  0.051
_exptl_absorpt_correction_T_min  0.025
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details
;with the help of the X-SHAPE soft ware by STOE, based on the program HABITUS
 by W. Herrendorf, Univ. Giessen, 1995
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    7.006
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             1624
_exptl_crystal_size_max          0.11
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.08
_refine_diff_density_max         3.263
_refine_diff_density_min         -3.287
_refine_diff_density_rms         0.697
_refine_ls_extinction_coef       0.00012(7)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.181
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     44
_refine_ls_number_reflns         1312
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.181
_refine_ls_R_factor_all          0.0901
_refine_ls_R_factor_gt           0.0603
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0130P)^2^+91.5619P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0938
_refine_ls_wR_factor_ref         0.1032
_reflns_number_gt                1017
_reflns_number_total             1312
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            BaLu2Te4_Pnma_crystals-01-00078-s001_DC155.CIF
_cod_data_source_block           balu2te4_chateigner_1508410
_cod_depositor_comments          'mistake in journal volume'
_cod_original_sg_symbol_H-M      Pnma
_cod_database_code               1508410